Download Biodegradable plastic.pdf...
BIODEGRADABLE PLASTICS FROM CASSAVA STARCH IN THAILAND 1
Klanarong Sriroth , Rungsima Chollakup Chollakup , Kuakoon Piyachomkwan and Christopher G. Oates 3
ABSTRACT The paper reviews the role of starch and biodegradable plastics production in Thailand, emphasizing the potential contribution of cassava starch in these products. Types of biodegradable plastics and their manufacturing processes are described. The major types of biodegradable plastics discussed are directly-expanded starch products and various starch-polymer blends (PCL, PLA, PVA and PHA). Research focusing on cassava starch incorporation into biodegradable plastics is summarized.
INTRODUCTION The world production of plastic is estimated to be more than 100 million tonnes per year. The need for such large quantities of conventional conventional plastics and their dominance dominance over other materials is due due to their excellent “long-life” “long-life” properties. These properties include include resistance to chemical reactions, specially specially enzymatic reactions. For example, it can take up to one hundred years to degrade only a few grams of plastic (such as polyethylene) under normal environmental conditions. Degradation at high temperature, such as in pyrolysis (burning) tends to cause cause emission of toxic fumes. Plastic accumulation in the environment environment thus creates tremendous problems problems for the world, presently and in the future. Environmental problems caused by plastics include changes to the carbon dioxide cycle, problems in composting, and increased increased toxic toxic emissions. emissions. Stimulated by environmental environmental concerns, scientists are now concentrating concentrating on ways to develop plastic plastic use more efficiently. Two simple strategies are to “recycle” (reuse), or to produce plastics that will degrade when no longer required.
Degradable plastics are grouped by the American Society for Testing and Materials (ASTM D20.96) as: a) Photodegradable plastics – A degradable plastic in which the degradation results from the action of natural daylight; b) Oxidatively degradable plastics – A degradable plastic in which the degradation results from oxidation; c) Hydrolytically degradable plastics – A degradable plastic in which the degradation results from hydrolysis; and d) Biodegradable plastics – A degradable plastic in which the degradation results from the action of naturally occurring microorganisms such as bacteria, fungi and algae. As the plastics defined in categories a), b) and c) require additional inputs, such as light (UV) or oxygen for degradation, the biodegradable plastics (d) offer the only products which are “naturally” degradable. 1
Department of Biotechnology, Kasetsart University, Bangkok, Thailand. National Center for Genetic Engineering and Biotechnology (BIOTEC), Bangkok, Thailand. 3 Agro Food Resources (Thailand) Co., Ltd. 2
Biodegradable plastics are polymers or polymer blends, which in addition to possessing properties similar to conventional plastics are susceptible to “natural” enzyme hydrolysis or other chemical attack. The plastic is therefore either broken down to oligosaccharides or monomers, through “depolymerization”, or are degraded to gaseous components through mineralization. Starch, a natural polymer, is biodegradable and as such can play an important role in the biodegradable plastic manufacturing process. It is also inexpensive and renewable. In tropical countries cassava starch offers opportunities due to its purity, clearness of its paste and low cost of production. This starch also posseses properties that enable it to be blended with other expensive polymers required for producing biodegradable plastic. Projections for the requirement of biodegradable plastic, by the year 2000, is 1.68 million tonnes (Table 1). Table 1. Projections of world consumption of biodegradable plastics in the year 2000.
Quantity (million tonnes)
Trash bags Agricultural Food containers/utensils One–way packaging Food packaging Total
1.00 0.09 0.18 0.27 0.14 1.68
Source: Chemical Week , October 27, 1993.
The “Cradle–To–Grave” concept ( Figure 1) has been designed by the Michigan Biotechnology Institute (1994). As the end use of products from biodegradable plastic is composting, it can serve as a reserve for carbon dioxide and as a means to return nutrients back to the soil (as compost). MANUFACTURING PROCESS TECHNOLOGY 1. Starch Puff This kind of product is known also as “Gelatinized starch puff” or “Plate expanded by extrusion” or “Baking with water”. The products are formed by the swelling and expansion of starch through the action of high temperature and water vapor. The products formed in the extruder are starch foam, snack, etc ( Figures 2 and 3). Plate expansion or baking give products such as waffles, which can be formed in tray shapes or other packaging material.
Clean Green Company in Minneapolis, MN, USA, has produced “starch foam” called “peanut” (American name of loose fill packing material) by extrusion of wheat starch (90 portion) and polyvinyl alcohol (10 portion). “Eco–Foam”, a product of National Starch, uses waxy corn as raw material. In European countries, the baking technology is also at a commercial scale. Packaging products, such as fast food utensils, are available in the market using both cereal and potato starches. The marketing of biodegradable packaging products are supported in the EU.
Figure 1. Design concept of biodegradable plastic “from cradle to grave”. Source: Michigan Biotechnology Institute, 1994.
high pressure high temperature controlled moisture content
Cassava foams Figure 2. Extrusion of starch foam.
Figure 3. Starch foam: (a) Pesika Naturpack GmbH; (b) Suedstraerke GmbH.
Cassava starch has been successfully expanded under extrusion conditions. Due to its low bulk density, a little modification is needed so that its moisture content is increased. Twin screw extrusion is recommended for direct expansion of cassava starches. Cassava starch can also be used as the raw material for plate expanded or baking products. Cassava starch can be expanded in moulds, at 200-240 °C for 1-3 minutes, to form into package utensils, such as bowls. About 10% additives, including calcium carbonate, agar, or emulsifier are needed to improve the properties. The bulk density is reported in the range of 0.15 to 0.176 g/cm3 (Poovarodom and Praditduang, 1999) Even though this group of products has been introduced to the market for some time, and can be produced at reasonable cost, constraints to its wider adoption still exist. First, special machinery is required, such as high shear extruder (not plastic extruder), continuous molding machine with high temperature (continuous waffle moulds using high pressure and temperature). Thus, the investment cost for the machinery is high. Distribution of the products is limited, due to its rigidity and short shelf life. Further, these products can not be applied to high moisture conditions. Lamination with other polymers, to improve shelf life and tolerance to high moisture conditions, will increase production cost, and such polymers have to be approved before using as a food packaging material. 2. Polymer/Starch Blends The biodegradable polymers (polylactic acid, polyhydroxyl butyrate) are in this group produced by fermentation (using starch hydrolysis products: glucose, maltose, etc.). The blending of polymers with starch under controlled conditions leads to co polymerization that in turn results in high molecular polymers with thermoplastic properties. Though the mixing or blending needs special machinery, such as an extruder, the products (polymer blend) can be handled as easily as conventional plastic resin.
Polymer blends can be distributed or transported to normal plastic converters, which can process the blends to products using normal injection or blow moulds. 2.1 Polymers Though starch, such as that of cassava, is used as a polymer, other polymers are frequently used in the blend: a. Polycaprolactone
Mn = 4x104
Tm = 62oC
This polyester is manufactured by catalytic ring-opening polymerization of εcaprolactone. Union Carbide is the biggest manufacturer ( Table 2). Polycaprolactone blend is the most used polymer/starch blend because of its low melting temperature (Tm) and high susceptibility to amylase and lipase hydrolyses (Tokiwa et al., 1990a; 1990b). A number of patents of polycaprolactone/starch blend are held: - Michigan Biotechnology International (MBI), USA (US 5,578,691 etc.) - Chuo Kajuku Co., Ltd, Japan (US 5,256,711 etc) - Bioplastics Inc., Suite, Ml. - Daicel Chemical Industries Co., Ltd, Japan - Japan Corn Starch, Japan Most patents describe a generic starch, this includes cassava. b. Polylactic acid
Mn = 1.88 x 10 5
Tm = 175oC
This polyester is manufactured by catalytic ring-opening polymerization of lactide (dilactone of lactic acid). Cargill, Minneapolis, MN, USA is the biggest manufacturer (Table 2). Polylactic acid is used because lactic acid can be produced by microorganisms
through a fermentation process. Many research laboratories in Japan claim that polylactic acid can be produced from a condensation-polymerization reaction of free lactic acid (from fermentation of starch). Polylactic acid from direct condensation polymerization is on the market under the names of “Lacty” (Shimadzu Corp. Japan) and “Lacea” (Mitsui Chemicals, Japan). These products offers the opportunity for a polymer blend totally derived from starch-based materials. - Polybutylene succinate (PBS), and - Polybutylene succinate/adipate (PBSA)
Mn = 3x10
Tm = 96 C
These products are derived from polycondensation of linear dicarboxylic acid with glycols. In the market they are sold under the name of “Bionolle” (Showa Highpolymer Inc., Japan); a wide range of molecular weights and properties are available. c.
Polyvinyl alcohol (PVA)
OH OH - CH 2 - CH - CH 2 - CH Mn = 7x10
Tm = 180 C
This is one of the most common synthetic polymers which can be easily biodegraded (Sakai et al., 1987). However due to its solubility, applications are limited. d. Polyhydroxyalkanoates (PHA)
This group of products are obtained from microorganisms through a fermentation process. Properties can be thermoplastic to elastomeric depending on the monomers used. The most popular product of this group is poly (3–hydroxybutyrate) (PHV). The manufacturers and prices of polymers are shown in Table 2.
Table 2. Manufacturers, capacity and cost of biodegradable polymers.
Cost ( $/lb)
Cargill, Minneapolis, MN
Ecochem, Wilmington, DE
Zeneca (business unit of ICI)
Renewable resources, Maize Renewable resources, Cheese whey, Maize Renewable resources, Carbohydrates (glucose), organic acids Renewable resources Petrochemical
Novamont, Montedison, Italy